2. 605 Large Diameter Carbon Steel Flanges
2.5 MSS Standard:7
MSS SP-25 Standard Marking System for Valves, Fittings,
Flanges, and Unions
3. General Requirements and Ordering Information
3.1 Product furnished to this speciﬁcation shall conform to
the requirements of Speciﬁcation A 961/A 961M, including
any supplementary requirements that are indicated in the
purchase order. Failure to comply with the requirements of
Speciﬁcation A 961/A 961M constitutes nonconformance with
this speciﬁcation. In case of a conﬂict between the require-
ments of this speciﬁcation and Speciﬁcation A 961/A 961M,
this speciﬁcation shall prevail.
3.2 It is the purchaser’s responsibility to specify in the
purchase order all ordering information necessary to purchase
the needed material. Examples of such information include but
are not limited to the following:
3.2.1 Additional requirements (see 15.1 and 15.2).
4. Materials and Manufacture
4.1 The steel shall be made by one or more of the following
processes: open-hearth, basic-oxygen, or electric-furnace, and
shall be fully killed, ﬁne-grain practice.
4.2 Forgings shall be manufactured from ingots, blooms,
billets, slabs, or bars. These items shall be forged, rolled, or
4.3 A sufficient discard shall be made from the ingot to
secure freedom from injurious piping and undue segregation.
4.4 The ﬁnished product shall be a forging as deﬁned by the
Terminology section of Speciﬁcation A 788/A 788M.
5. Heat Treatment
5.1 Following plastic working, the forging manufacturer
shall heat treat the forgings by normalizing, or normalizing and
tempering, or quenching and tempering.
5.1.1 Normalizing—The procedure for normalizing shall
consist of uniformly heating the forgings to a temperature
between 1550 and 1700 °F [845 and 925 °C], holding a
sufficient time to attain uniform temperature throughout, and
cooling in still air. The forging shall be at a temperature below
1000 °F [540 °C] before heating for normalizing.
5.1.2 Quenching—The procedure for quenching shall con-
sist of uniformly heating the forging to a temperature between
1550 and 1700 °F [845 and 925 °C], holding a sufficient time
to attain uniform temperature throughout, and quenching into a
suitable liquid medium. The forging shall be at a temperature
below 1000 °F [540 °C] before heating for quenching.
5.1.3 Tempering—The procedure for tempering shall con-
sist of reheating the forging subsequent to normalizing or
quenching to a temperature of at least 1100 °F [595 °C], but not
above the lower transformation temperature, for 30 min/in. [30
min/25 mm] of maximum section thickness, with minimum
holding time at tempering temperature not less than 30 min.
6. Chemical Composition
6.1 The steel shall conform to the requirements as to
chemical composition prescribed in Table 1.
6.2 Steels to which lead has been added shall not be used.
7. Mechanical Requirements Mechanical Requirements
7.1 Tension Tests:
7.1.1 Requirements—The material shall conform to require-
ments for tensile properties prescribed in Table 2.
184.108.40.206 The test specimen shall be obtained from a rough or
ﬁnished production forging, or prolongation thereof, or it may
be obtained from separately forged test blanks from the same
heat of steel as the production forging. The test blank shall be
reduced by forging in a manner similar to that for the products
represented, shall receive approximately the same hot working
and reduction, be of the same nominal thickness, and receive
the same heat treatment as the ﬁnished products represented.
The test material shall be treated in the same furnace at the
same time as the forging it represents, subject to the require-
ments of 220.127.116.11.
7.1.2 Number of Tests—One tension test at room tempera-
ture shall be made for each nominal wall thickness 6 1⁄4 in.
[6 6 mm] from each heat in each heat treatment charge.
18.104.22.168 If heat treatment is performed in either a continuous
or a batch-type furnace controlled within 6 25 °F [6 14 °C] of
the required heat-treatment temperature, and equipped with
Available from Manufacturers Standardization Society of the Valve and Fittings
Industry (MSS), 127 Park St., NE, Vienna, VA 22180-4602, http://www.mss-
TABLE 1 Chemical Requirements
Elements Composition, %
Heat Analysis 0.25 max
Product Analysis 0.28 max
Heat Analysis 0.90 to 1.35
Product Analysis 0.84 to 1.41
Heat Analysis 0.035 max
Product Analysis 0.043 max
Heat Analysis 0.025 max
Product Analysis 0.033 max
Heat Analysis 0.15 to 0.30
Product Analysis 0.13 to 0.32
Heat Analysis 0.40A
Product Analysis 0.43
Heat Analysis 0.30A,B
Product Analysis 0.34
Heat Analysis 0.12A,B
Product Analysis 0.13
Heat Analysis 0.40A
Product Analysis 0.43
Heat Analysis 0.02
Product Analysis 0.03
Heat Analysis 0.05
Product Analysis 0.055
The sum of copper, nickel, chromium and molybdenum shall not exceed
1.00 % on heat analysis.
The sum of chromium and molybdenum shall not exceed 0.32 % on heat
A 727/A 727M – 02 (2007)
3. recording pyrometers so that complete records of heat treat-
ment are available and if the same heat treating cycles are used
on the forgings represented by the tension test, then one tension
test per nominal wall thickness 6 1⁄4 in. [6 6 mm] from each
heat shall be required, instead of one tension test per nominal
wall thickness from each heat in each heat-treatment charge.
7.1.3 Test Locations and Orientations—The test specimen
shall be removed from the midwall of the heaviest section of
the forging or test blank.
22.214.171.124 The test specimen shall have its longitudinal axis
located parallel to the direction of major working of the forging
or test blank, except for ﬂanges and rings the test specimen
shall be in the tangential direction.
7.1.4 Test Method—Testing shall be performed in accor-
dance with Test Methods and Deﬁnitions A 370 using the
largest feasible of the round specimens. The gage length for
measuring elongation shall be four times the diameter of the
7.2 Hardness Test:
7.2.1 Requirements—If the production forgings are liquid-
quenched and tempered, hardness of the forgings shall not
exceed 187 HB after heat treatment. The purchaser may verify
that the requirement has been met by testing at any location on
the forgings provided such testing does not render the forgings
8. Heat Analysis
8.1 An analysis of each heat of steel shall be made from
samples taken preferably during the pouring of the heat. The
results shall conform to Table 1.
9. Product Analysis
9.1 A product analysis may be made by the purchaser on
samples taken in accordance with Practice E 59. The results
shall conform to Table 1.
10. Hydrostatic Test
10.1 Forgings manufactured under this speciﬁcation shall be
capable of passing a hydrostatic test compatible with the rating
of the ﬁnished forging. Such tests shall be conducted by the
forging manufacturer only when Supplementary Requirement
S8 in Speciﬁcation A 961/A 961M is speciﬁed.
11. Rework and Retreatment
11.1 If the results of mechanical tests do not conform to the
requirements speciﬁed, the manufacturer may reheat treat the
forgings represented, and shall retest to the applicable require-
11.2 Individually tested forgings meeting all requirements
shall be acceptable.
12. Repair by Welding
12.1 Repair of defects by welding shall be permitted at the
discretion of the forging manufacturer.
12.2 Repair by welding shall be made using welding pro-
cedures and welders qualiﬁed in accordance with Section IX of
the ASME Boiler and Pressure Vessel Code. When forgings are
heat treated after repair welding, the qualiﬁcation test plates
shall be subjected to the same heat treatment. The mechanical
properties of the qualiﬁcation test plates shall conform to
12.3 Only electrode classiﬁcations with the -A1 designator
shall be used (for example, E71T1-A1). SMAW, GMAW,
FCAW or GTAW may be used. The GMAW process is limited
to either the spray transfer or pulsed arc process. The FCAW
process is limited to repair of carbon or carbon-molybdenum
base materials only. Electrodes shall conform to the applicable
AWS A5 electrode speciﬁcation.
12.4 Forgings repair welded in the normalized, normalized
and tempered, or the quenched and tempered conditions shall
be stress-relieved after repair welding at 1100 °F [595 °C]
minimum, but not higher than the temperature previously used
for tempering the base metal of the same forging, or shall be
reheat treated in accordance with Section 5.
13.1 All tests and inspections shall be made at the place of
manufacture, unless otherwise agreed, except for product
analysis (see 9.1).
14. Rejection and Rehearing
14.1 Each forging that develops injurious defects during
shop working or application shall be rejected and the manu-
15.1 For forgings made to speciﬁed dimensions, when
agreed to by the purchaser, and for forgings made to dimen-
sional standards, application of identiﬁcation marks as required
in Section 16 shall be the certiﬁcation that the forgings have
been furnished in accordance with the requirements of this
15.2 When test reports are required, they shall include
certiﬁcation that all requirements of this speciﬁcation have
been met. The reports shall show the results of all required
tests, the heat number or manufacturer’s heat identiﬁcation, a
description of the heat treatment used, and shall be traceable to
the forging represented. The speciﬁcation designation included
on test reports shall include year of issue and revision letter, if
16. Product Marking
16.1 Identiﬁcation marks consisting of the speciﬁcation
designation, manufacturer’s name or symbol, (Note 2) the heat
number or manufacturer’s heat identiﬁcation, size, and service
rating, if applicable, shall be permanently placed on each
forging in a position that will not affect the usefulness of the
forging. When size does not permit complete marking, identi-
ﬁcation marks may be omitted in the sequence speciﬁed in
TABLE 2 Tensile Requirements
Tensile strength, ksi [MPa] 60.0 to 85.0 [415 to 585]
Yield strength, min, ksi [MPa]A
Elongation in 2 in. or 50 mm, min, % 22
Reduction of area, min, % 30
Determined by either the 0.2 % offset method or the 0.5 % extension-under-
A 727/A 727M – 02 (2007)
4. SP-25, except that the word “steel” shall not be substituted for
the speciﬁcation designation. The speciﬁcation number marked
on the forgings need not include speciﬁcation year of issue and
NOTE 2—For purposes of identiﬁcation marking, the manufacturer is
considered the organization that certiﬁes the piping component was
manufactured, sampled, and tested in accordance with this speciﬁcation
and the results have been determined to meet the requirements of this
16.1.1 If the forgings have been quenched and tempered the
letters “QT” shall be stamped on the forgings following the
16.1.2 Forgings repaired by welding shall be marked with
the letter “W” following the speciﬁcation designation.
16.2 When test reports are required, additional marks shall
be used as necessary to identify the part with the test report.
16.3 Bar Coding—In addition to the requirements in 16.1
and 16.2, bar coding is acceptable as a supplemental identiﬁ-
cation method. The purchaser may specify in the order a
speciﬁc bar coding system to be used. The bar coding system,
if applied at the discretion of the supplier, should be consistent
with one of the published industry standards for bar coding. If
used on small parts, the bar code may be applied to the box or
a substantially applied tag.
17.1 carbon equivalent; pipe ﬁttings; steel; piping applica-
tions; pressure containing parts; steel ﬂanges; steel forgings;
carbon; steel valves; temperature service applications; low
One or more of the following supplementary requirements shall be applied only when speciﬁed by
the purchaser in the inquiry, contract, or order. Details of these supplementary requirements shall be
agreed upon in writing by the manufacturer and purchaser. Supplementary requirements shall in no
way negate any requirement of the speciﬁcation.
S1. Carbon Equivalent
S1.1 The maximum carbon equivalent, based on heat analy-
sis shall be 0.45 for forgings with a maximum section thickness
of 2 in. or less, and 0.46 for forgings with a maximum section
thickness of greater than 2 in.
S1.2 Determine the carbon equivalent (CE) as follows:
CE = C + Mn/6 + (Cr + Mo + V)/5 + (Ni + Cu)/15
S1.3 A lower maximum carbon equivalent may be agreed
upon between the supplier and the purchaser.
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned
in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk
of infringement of such rights, are entirely their own responsibility.
This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and
if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards
and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the
responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should
make your views known to the ASTM Committee on Standards, at the address shown below.
This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959,
United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above
address or at 610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website
A 727/A 727M – 02 (2007)